#------------------------------------------------------------------------------
#$Date: 2016-03-21 17:36:45 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178787 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/41/4104100.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4104100
loop_
_publ_author_name
'Irina P. Roof'
'Mark D. Smith'
'Sangmoon Park'
'Hans-Conrad zur Loye'
_publ_section_title
;
 EuKNaTaO5: Crystal Growth, Structure and Photoluminescence Property
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              4202
_journal_page_last               4203
_journal_paper_doi               10.1021/ja8100769
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'Eu K Na O5 Ta'
_chemical_formula_sum            'Eu K Na O5 Ta'
_chemical_formula_weight         475.00
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           129
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   5.6878(2)
_cell_length_b                   5.6878(2)
_cell_length_c                   8.2258(2)
_cell_measurement_reflns_used    3611
_cell_measurement_temperature    294(2)
_cell_measurement_theta_max      40.200
_cell_measurement_theta_min      4.356
_cell_volume                     266.113(15)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.625 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  'SHELXTL Version 6.14 (Bruker, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      294(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0291
_diffrn_reflns_av_sigmaI/netI    0.0175
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            6039
_diffrn_reflns_theta_full        40.23
_diffrn_reflns_theta_max         40.23
_diffrn_reflns_theta_min         2.48
_exptl_absorpt_coefficient_mu    33.015
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.3662
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    5.928
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             412
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.023
_refine_diff_density_min         -1.759
_refine_diff_density_rms         0.265
_refine_ls_extinction_coef       0.0034(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.168
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         531
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.168
_refine_ls_R_factor_all          0.0202
_refine_ls_R_factor_gt           0.0180
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0176P)²+0.3349P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0389
_refine_ls_wR_factor_ref         0.0401
_reflns_number_gt                499
_reflns_number_total             531
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja8100769_si_001.cif
_cod_data_source_block           ivp2001s
_cod_original_sg_symbol_H-M      'P 4/n m m'
_cod_database_code               4104100
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-y+1/2, x, z'
'y, -x+1/2, z'
'-x, y+1/2, -z'
'x+1/2, -y, -z'
'y+1/2, x+1/2, -z'
'-y, -x, -z'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'y-1/2, -x, -z'
'-y, x-1/2, -z'
'x, -y-1/2, z'
'-x-1/2, y, z'
'-y-1/2, -x-1/2, z'
'y, x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ta1 Ta 0.2500 0.2500 0.26047(3) 0.00765(7) Uani 1 8 d S
Eu1 Eu 0.7500 0.2500 0.5000 0.00868(7) Uani 1 8 d S
K1 K 0.7500 0.2500 0.0000 0.0252(4) Uani 1 8 d S
Na1 Na 0.2500 0.2500 0.7598(3) 0.0104(5) Uani 1 8 d S
O1 O 0.0186(3) 0.0186(3) 0.3314(3) 0.0124(4) Uani 1 2 d S
O2 O 0.2500 0.2500 0.0369(6) 0.0160(8) Uani 1 8 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Ta1 O1 107.39(7) . .
O2 Ta1 O1 107.40(7) . 3
O1 Ta1 O1 84.87(4) . 3
O2 Ta1 O1 107.40(7) . 4
O1 Ta1 O1 84.87(4) . 4
O1 Ta1 O1 145.21(14) 3 4
O2 Ta1 O1 107.40(7) . 2
O1 Ta1 O1 145.21(14) . 2
O1 Ta1 O1 84.87(4) 3 2
O1 Ta1 O1 84.87(4) 4 2
O2 Ta1 Eu1 124.72(1) . 1_455
O1 Ta1 Eu1 43.54(4) . 1_455
O1 Ta1 Eu1 112.61(6) 3 1_455
O1 Ta1 Eu1 43.54(4) 4 1_455
O1 Ta1 Eu1 112.61(6) 2 1_455
O2 Ta1 Eu1 124.72(1) . 9_656
O1 Ta1 Eu1 43.54(4) . 9_656
O1 Ta1 Eu1 43.54(4) 3 9_656
O1 Ta1 Eu1 112.61(6) 4 9_656
O1 Ta1 Eu1 112.61(6) 2 9_656
Eu1 Ta1 Eu1 71.075(3) 1_455 9_656
O2 Ta1 Eu1 124.72(1) . .
O1 Ta1 Eu1 112.61(6) . .
O1 Ta1 Eu1 43.54(4) 3 .
O1 Ta1 Eu1 112.61(6) 4 .
O1 Ta1 Eu1 43.54(4) 2 .
Eu1 Ta1 Eu1 110.569(6) 1_455 .
Eu1 Ta1 Eu1 71.075(3) 9_656 .
O2 Ta1 Eu1 124.72(1) . 9_666
O1 Ta1 Eu1 112.61(6) . 9_666
O1 Ta1 Eu1 112.61(6) 3 9_666
O1 Ta1 Eu1 43.54(4) 4 9_666
O1 Ta1 Eu1 43.54(4) 2 9_666
Eu1 Ta1 Eu1 71.075(3) 1_455 9_666
Eu1 Ta1 Eu1 110.570(6) 9_656 9_666
Eu1 Ta1 Eu1 71.075(3) . 9_666
O2 Ta1 K1 53.01(1) . 1_455
O1 Ta1 K1 68.96(6) . 1_455
O1 Ta1 K1 135.96(4) 3 1_455
O1 Ta1 K1 68.96(6) 4 1_455
O1 Ta1 K1 135.96(4) 2 1_455
Eu1 Ta1 K1 71.71(1) 1_455 1_455
Eu1 Ta1 K1 110.041(1) 9_656 1_455
Eu1 Ta1 K1 177.721(6) . 1_455
Eu1 Ta1 K1 110.041(1) 9_666 1_455
O2 Ta1 K1 53.01(1) . 9_655
O1 Ta1 K1 68.96(6) . 9_655
O1 Ta1 K1 68.96(6) 3 9_655
O1 Ta1 K1 135.96(4) 4 9_655
O1 Ta1 K1 135.96(4) 2 9_655
Eu1 Ta1 K1 110.041(1) 1_455 9_655
Eu1 Ta1 K1 71.71(1) 9_656 9_655
Eu1 Ta1 K1 110.040(1) . 9_655
Eu1 Ta1 K1 177.721(6) 9_666 9_655
K1 Ta1 K1 68.772(3) 1_455 9_655
O2 Ta1 K1 53.01(1) . .
O1 Ta1 K1 135.96(4) . .
O1 Ta1 K1 68.96(6) 3 .
O1 Ta1 K1 135.96(4) 4 .
O1 Ta1 K1 68.96(6) 2 .
Eu1 Ta1 K1 177.721(6) 1_455 .
Eu1 Ta1 K1 110.040(1) 9_656 .
Eu1 Ta1 K1 71.71(1) . .
Eu1 Ta1 K1 110.040(1) 9_666 .
K1 Ta1 K1 106.012(6) 1_455 .
K1 Ta1 K1 68.772(3) 9_655 .
O1 Eu1 O1 69.51(9) 3 11_656
O1 Eu1 O1 65.06(9) 3 2
O1 Eu1 O1 108.74(5) 11_656 2
O1 Eu1 O1 108.74(5) 3 9_656
O1 Eu1 O1 65.06(9) 11_656 9_656
O1 Eu1 O1 172.99(10) 2 9_656
O1 Eu1 O1 108.74(5) 3 10_666
O1 Eu1 O1 77.25(10) 11_656 10_666
O1 Eu1 O1 69.51(9) 2 10_666
O1 Eu1 O1 110.95(9) 9_656 10_666
O1 Eu1 O1 77.25(10) 3 1_655
O1 Eu1 O1 108.74(5) 11_656 1_655
O1 Eu1 O1 110.95(9) 2 1_655
O1 Eu1 O1 69.51(9) 9_656 1_655
O1 Eu1 O1 172.99(10) 10_666 1_655
O1 Eu1 O1 172.99(9) 3 12_666
O1 Eu1 O1 110.95(9) 11_656 12_666
O1 Eu1 O1 108.74(5) 2 12_666
O1 Eu1 O1 77.25(10) 9_656 12_666
O1 Eu1 O1 65.06(9) 10_666 12_666
O1 Eu1 O1 108.74(5) 1_655 12_666
O1 Eu1 O1 110.95(9) 3 4_655
O1 Eu1 O1 172.99(9) 11_656 4_655
O1 Eu1 O1 77.25(10) 2 4_655
O1 Eu1 O1 108.74(5) 9_656 4_655
O1 Eu1 O1 108.74(5) 10_666 4_655
O1 Eu1 O1 65.06(9) 1_655 4_655
O1 Eu1 O1 69.51(9) 12_666 4_655
O1 Eu1 Ta1 33.30(5) 3 .
O1 Eu1 Ta1 83.15(5) 11_656 .
O1 Eu1 Ta1 33.30(5) 2 .
O1 Eu1 Ta1 139.89(5) 9_656 .
O1 Eu1 Ta1 83.15(5) 10_666 .
O1 Eu1 Ta1 100.97(5) 1_655 .
O1 Eu1 Ta1 139.89(5) 12_666 .
O1 Eu1 Ta1 100.97(5) 4_655 .
O1 Eu1 Ta1 83.15(5) 3 9_656
O1 Eu1 Ta1 33.30(5) 11_656 9_656
O1 Eu1 Ta1 139.89(5) 2 9_656
O1 Eu1 Ta1 33.30(5) 9_656 9_656
O1 Eu1 Ta1 100.97(5) 10_666 9_656
O1 Eu1 Ta1 83.15(5) 1_655 9_656
O1 Eu1 Ta1 100.97(5) 12_666 9_656
O1 Eu1 Ta1 139.89(5) 4_655 9_656
Ta1 Eu1 Ta1 108.925(3) . 9_656
O1 Eu1 Ta1 139.89(5) 3 9_666
O1 Eu1 Ta1 100.97(5) 11_656 9_666
O1 Eu1 Ta1 83.15(5) 2 9_666
O1 Eu1 Ta1 100.97(5) 9_656 9_666
O1 Eu1 Ta1 33.30(5) 10_666 9_666
O1 Eu1 Ta1 139.89(5) 1_655 9_666
O1 Eu1 Ta1 33.30(5) 12_666 9_666
O1 Eu1 Ta1 83.15(5) 4_655 9_666
Ta1 Eu1 Ta1 108.925(3) . 9_666
Ta1 Eu1 Ta1 110.569(6) 9_656 9_666
O1 Eu1 Ta1 100.97(5) 3 1_655
O1 Eu1 Ta1 139.89(5) 11_656 1_655
O1 Eu1 Ta1 100.97(5) 2 1_655
O1 Eu1 Ta1 83.15(5) 9_656 1_655
O1 Eu1 Ta1 139.89(5) 10_666 1_655
O1 Eu1 Ta1 33.30(5) 1_655 1_655
O1 Eu1 Ta1 83.15(5) 12_666 1_655
O1 Eu1 Ta1 33.30(5) 4_655 1_655
Ta1 Eu1 Ta1 110.569(7) . 1_655
Ta1 Eu1 Ta1 108.925(3) 9_656 1_655
Ta1 Eu1 Ta1 108.925(3) 9_666 1_655
O2 K1 O2 90.65(2) 9_655 .
O2 K1 O2 90.65(2) 9_655 1_655
O2 K1 O2 167.82(19) . 1_655
O2 K1 O2 167.82(19) 9_655 9_665
O2 K1 O2 90.65(2) . 9_665
O2 K1 O2 90.64(2) 1_655 9_665
O2 K1 O1 57.77(9) 9_655 11_655
O2 K1 O1 72.50(9) . 11_655
O2 K1 O1 118.12(8) 1_655 11_655
O2 K1 O1 111.27(9) 9_665 11_655
O2 K1 O1 72.50(9) 9_655 3
O2 K1 O1 57.77(9) . 3
O2 K1 O1 111.27(9) 1_655 3
O2 K1 O1 118.12(8) 9_665 3
O1 K1 O1 107.25(5) 11_655 3
O2 K1 O1 57.77(9) 9_655 9_655
O2 K1 O1 118.12(8) . 9_655
O2 K1 O1 72.50(9) 1_655 9_655
O2 K1 O1 111.27(9) 9_665 9_655
O1 K1 O1 45.68(6) 11_655 9_655
O1 K1 O1 130.26(3) 3 9_655
O2 K1 O1 118.12(8) 9_655 2
O2 K1 O1 57.77(9) . 2
O2 K1 O1 111.27(9) 1_655 2
O2 K1 O1 72.50(9) 9_665 2
O1 K1 O1 130.26(3) 11_655 2
O1 K1 O1 45.68(6) 3 2
O1 K1 O1 174.94(7) 9_655 2
O2 K1 O1 72.50(9) 9_655 1_655
O2 K1 O1 111.27(9) . 1_655
O2 K1 O1 57.77(9) 1_655 1_655
O2 K1 O1 118.12(8) 9_665 1_655
O1 K1 O1 130.26(3) 11_655 1_655
O1 K1 O1 53.56(6) 3 1_655
O1 K1 O1 107.24(5) 9_655 1_655
O1 K1 O1 72.99(5) 2 1_655
O2 K1 O1 111.27(9) 9_655 10_665
O2 K1 O1 72.50(9) . 10_665
O2 K1 O1 118.12(8) 1_655 10_665
O2 K1 O1 57.77(9) 9_665 10_665
O1 K1 O1 53.56(6) 11_655 10_665
O1 K1 O1 130.26(3) 3 10_665
O1 K1 O1 72.99(5) 9_655 10_665
O1 K1 O1 107.24(5) 2 10_665
O1 K1 O1 174.94(7) 1_655 10_665
O2 K1 O1 118.12(8) 9_655 4_655
O2 K1 O1 111.27(9) . 4_655
O2 K1 O1 57.77(9) 1_655 4_655
O2 K1 O1 72.50(9) 9_665 4_655
O1 K1 O1 174.94(7) 11_655 4_655
O1 K1 O1 72.99(5) 3 4_655
O1 K1 O1 130.26(3) 9_655 4_655
O1 K1 O1 53.56(6) 2 4_655
O1 K1 O1 45.68(6) 1_655 4_655
O1 K1 O1 130.26(3) 10_665 4_655
O2 K1 O1 111.27(9) 9_655 12_665
O2 K1 O1 118.12(8) . 12_665
O2 K1 O1 72.50(9) 1_655 12_665
O2 K1 O1 57.77(9) 9_665 12_665
O1 K1 O1 72.99(5) 11_655 12_665
O1 K1 O1 174.94(7) 3 12_665
O1 K1 O1 53.56(6) 9_655 12_665
O1 K1 O1 130.26(3) 2 12_665
O1 K1 O1 130.26(3) 1_655 12_665
O1 K1 O1 45.68(6) 10_665 12_665
O1 K1 O1 107.24(5) 4_655 12_665
O2 Na1 O1 109.13(8) 1_556 9_556
O2 Na1 O1 109.13(8) 1_556 12_566
O1 Na1 O1 83.83(5) 9_556 12_566
O2 Na1 O1 109.13(8) 1_556 11_656
O1 Na1 O1 83.83(5) 9_556 11_656
O1 Na1 O1 141.73(17) 12_566 11_656
O2 Na1 O1 109.13(8) 1_556 10_666
O1 Na1 O1 141.73(17) 9_556 10_666
O1 Na1 O1 83.83(5) 12_566 10_666
O1 Na1 O1 83.83(5) 11_656 10_666
O2 Na1 K1 55.21(3) 1_556 1_456
O1 Na1 K1 68.80(5) 9_556 1_456
O1 Na1 K1 68.80(5) 12_566 1_456
O1 Na1 K1 137.36(5) 11_656 1_456
O1 Na1 K1 137.36(5) 10_666 1_456
O2 Na1 K1 55.21(3) 1_556 9_656
O1 Na1 K1 68.80(5) 9_556 9_656
O1 Na1 K1 137.36(5) 12_566 9_656
O1 Na1 K1 68.80(5) 11_656 9_656
O1 Na1 K1 137.36(5) 10_666 9_656
K1 Na1 K1 71.00(3) 1_456 9_656
O2 Na1 K1 55.21(3) 1_556 1_556
O1 Na1 K1 137.36(5) 9_556 1_556
O1 Na1 K1 137.36(5) 12_566 1_556
O1 Na1 K1 68.80(5) 11_656 1_556
O1 Na1 K1 68.80(5) 10_666 1_556
K1 Na1 K1 110.41(7) 1_456 1_556
K1 Na1 K1 71.00(3) 9_656 1_556
O2 Na1 K1 55.21(3) 1_556 9_666
O1 Na1 K1 137.36(5) 9_556 9_666
O1 Na1 K1 68.80(5) 12_566 9_666
O1 Na1 K1 137.36(5) 11_656 9_666
O1 Na1 K1 68.80(5) 10_666 9_666
K1 Na1 K1 71.00(3) 1_456 9_666
K1 Na1 K1 110.41(7) 9_656 9_666
K1 Na1 K1 71.00(3) 1_556 9_666
O2 Na1 Eu1 126.92(3) 1_556 9_656
O1 Na1 Eu1 43.03(4) 9_556 9_656
O1 Na1 Eu1 109.71(9) 12_566 9_656
O1 Na1 Eu1 43.03(4) 11_656 9_656
O1 Na1 Eu1 109.71(9) 10_666 9_656
K1 Na1 Eu1 110.046(3) 1_456 9_656
K1 Na1 Eu1 71.714(3) 9_656 9_656
K1 Na1 Eu1 110.046(3) 1_556 9_656
K1 Na1 Eu1 177.87(7) 9_666 9_656
O2 Na1 Eu1 126.92(3) 1_556 1_455
O1 Na1 Eu1 43.03(4) 9_556 1_455
O1 Na1 Eu1 43.03(4) 12_566 1_455
O1 Na1 Eu1 109.71(9) 11_656 1_455
O1 Na1 Eu1 109.71(9) 10_666 1_455
K1 Na1 Eu1 71.714(3) 1_456 1_455
K1 Na1 Eu1 110.046(3) 9_656 1_455
K1 Na1 Eu1 177.87(7) 1_556 1_455
K1 Na1 Eu1 110.046(3) 9_666 1_455
Eu1 Na1 Eu1 68.85(3) 9_656 1_455
O2 Na1 Eu1 126.92(3) 1_556 .
O1 Na1 Eu1 109.71(9) 9_556 .
O1 Na1 Eu1 109.71(9) 12_566 .
O1 Na1 Eu1 43.03(4) 11_656 .
O1 Na1 Eu1 43.03(4) 10_666 .
K1 Na1 Eu1 177.87(7) 1_456 .
K1 Na1 Eu1 110.046(3) 9_656 .
K1 Na1 Eu1 71.713(3) 1_556 .
K1 Na1 Eu1 110.046(2) 9_666 .
Eu1 Na1 Eu1 68.85(3) 9_656 .
Eu1 Na1 Eu1 106.16(6) 1_455 .
Ta1 O1 Na1 143.47(14) . 9_556
Ta1 O1 Eu1 103.17(6) . 1_455
Na1 O1 Eu1 97.35(7) 9_556 1_455
Ta1 O1 Eu1 103.17(6) . 9_656
Na1 O1 Eu1 97.35(7) 9_556 9_656
Eu1 O1 Eu1 110.49(9) 1_455 9_656
Ta1 O1 K1 78.57(6) . 1_455
Na1 O1 K1 72.23(7) 9_556 1_455
Eu1 O1 K1 88.03(2) 1_455 1_455
Eu1 O1 K1 160.09(7) 9_656 1_455
Ta1 O1 K1 78.57(6) . 9_655
Na1 O1 K1 72.23(7) 9_556 9_655
Eu1 O1 K1 160.09(7) 1_455 9_655
Eu1 O1 K1 88.03(2) 9_656 9_655
K1 O1 K1 72.76(5) 1_455 9_655
Ta1 O2 Na1 180.0 . 1_554
Ta1 O2 K1 96.09(9) . 9_655
Na1 O2 K1 83.91(9) 1_554 9_655
Ta1 O2 K1 96.09(9) . 1_455
Na1 O2 K1 83.91(9) 1_554 1_455
K1 O2 K1 89.36(2) 9_655 1_455
Ta1 O2 K1 96.09(9) . .
Na1 O2 K1 83.91(9) 1_554 .
K1 O2 K1 89.35(2) 9_655 .
K1 O2 K1 167.82(19) 1_455 .
Ta1 O2 K1 96.09(9) . 9_665
Na1 O2 K1 83.91(9) 1_554 9_665
K1 O2 K1 167.82(19) 9_655 9_665
K1 O2 K1 89.35(2) 1_455 9_665
K1 O2 K1 89.35(2) . 9_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ta1 O2 1.839(5) .
Ta1 O1 1.950(2) .
Ta1 O1 1.951(2) 3
Ta1 O1 1.951(2) 4
Ta1 O1 1.951(2) 2
Ta1 Eu1 3.45975(15) 1_455
Ta1 Eu1 3.45975(15) 9_656
Ta1 Eu1 3.45976(16) .
Ta1 Eu1 3.45977(15) 9_666
Ta1 K1 3.56066(16) 1_455
Ta1 K1 3.56066(16) 9_655
Ta1 K1 3.56067(16) .
Eu1 O1 2.4476(14) 3
Eu1 O1 2.4476(14) 11_656
Eu1 O1 2.4476(14) 2
Eu1 O1 2.4476(14) 9_656
Eu1 O1 2.4476(14) 10_666
Eu1 O1 2.4476(14) 1_655
Eu1 O1 2.4476(14) 12_666
Eu1 O1 2.4476(14) 4_655
Eu1 Ta1 3.45976(15) 9_656
Eu1 Ta1 3.45978(15) 9_666
Eu1 Ta1 3.45978(15) 1_655
K1 O2 2.8600(5) 9_655
K1 O2 2.8600(5) .
K1 O2 2.8601(5) 1_655
K1 O2 2.8601(5) 9_665
K1 O1 3.391(2) 11_655
K1 O1 3.391(2) 3
K1 O1 3.391(2) 9_655
K1 O1 3.391(2) 2
K1 O1 3.391(2) 1_655
K1 O1 3.391(2) 10_665
K1 O1 3.391(2) 4_655
K1 O1 3.391(2) 12_665
Na1 O2 2.280(5) 1_556
Na1 O1 2.287(2) 9_556
Na1 O1 2.287(2) 12_566
Na1 O1 2.287(2) 11_656
Na1 O1 2.287(2) 10_666
Na1 K1 3.4630(14) 1_456
Na1 K1 3.4630(14) 9_656
Na1 K1 3.4631(14) 1_556
Na1 K1 3.4631(14) 9_666
Na1 Eu1 3.5572(15) 9_656
Na1 Eu1 3.5572(15) 1_455
O1 Na1 2.287(2) 9_556
O1 Eu1 2.4476(14) 1_455
O1 Eu1 2.4476(14) 9_656
O1 K1 3.391(2) 1_455
O1 K1 3.391(2) 9_655
O2 Na1 2.280(5) 1_554
O2 K1 2.8600(5) 9_655
O2 K1 2.8600(5) 1_455
O2 K1 2.8601(5) 9_665
